0103 - 5053 $6.00+0.00
#Present address: Instituto de Química, Campus Samambaia, UFG, CP 131, 74001-970 Goiânia - GO, Brazil
Pt-Cu/C and Pd Modiied Pt-Cu/C Electrocatalysts for the Oxygen Reduction
Reaction in Direct Methanol Fuel Cells
Emilia A. Carbonio, Flavio Colmati,# Eduardo G. Ciapina, Maristela E. Pereira and
Ernesto R. Gonzalez*
Instituto de Química de São Carlos, Universidade de São Paulo, CP 780, 13560-970 São Carlos-SP, Brazil
Neste trabalho, foram preparados diferentes eletrocatalisadores de Pt–Cu e de Pt–Cu modiicados com Pd, suportados em carbono por meio da redução química de precursores de Pt, Cu e Pd com borohidreto de sódio. A atividade eletrocatalítica frente à reação de redução de oxigênio foi estudada. A análise dos resultados de difração de raios X mostrou que há formação de liga. Com microscopia eletrônica de transmissão (TEM) foi observado que as nanopartículas metálicas estão bem distribuídas no suporte de carbono. Espectroscopia de absorção de raios X dispersiva (DXAS) foi empregada para compreender melhor as propriedades intrínsecas dos materiais. Os eletrocatalisadores foram caracterizados eletroquimicamente por voltametria cíclica em H2SO4 0.5 mol L
-1 e a atividade eletrocatalítica destes foi estudada por meio de experimentos em estado estacionário em células a combustível de metanol direto (DMFC). A introdução de Pd ocasionou um aumento da atividade dos catalisadores de Pt–Cu. O melhor desempenho da DMFC foi obtido usando como cátodo o catalisador da liga de Pt50Pd40Cu10/C tratado termicamente a 500 °C em atmosfera de H2/Ar.
In this work, different carbon supported Pt-Cu catalysts and Pd modiied Pt-Cu catalysts were prepared by chemical reduction of Pt, Cu and Pd precursors with sodium borohydride, and their electrocatalytic activity for the oxygen reduction reaction was studied. X-ray diffraction analysis indicated alloy formation. Transmission electron microscopy (TEM) showed that the metal nanoparticles are well-distributed on the carbon support. Dispersive X-ray absorption spectroscopy (DXAS) was used to achieve a better understanding of the intrinsic properties of the materials. The electrocatalysts were characterized electrochemically by cyclic voltammetry in 0.5 mol L-1 H
2SO4 and their electrochemical activity was studied with steady-state experiments in a direct methanol fuel cell (DMFC). The introduction of Pd led to an improvement of the catalytic activity of the Pt−Cu catalysts. The best performance in a DMFC was obtained using, as cathode, a Pt50Pd40Cu10/C alloy catalyst thermally treated at 500 oC in an H
Keywords: oxygen reduction reaction, electrocatalysis, DMFC, cathodes
Direct methanol fuel cells (DMFCs) are promising electrochemical energy converters for a variety of applications because of the system simplicity. The use of methanol as fuel has several advantages in comparison to hydrogen: it is a cheap liquid fuel, easily handled, transported and stored, with a high theoretical energy density.1 An additional advantage of DMFC is it does not
require complex humidiication and heat management
modules as in the hydrogen fed proton exchange membrane fuel cell (PEMFC) system. The dilute methanol/water mixture circulating around the DMFC provides the necessary humidiication and heat management.
One of the main problems of DMFC’s, which decreases the eficiency of conversion of the chemical energy of the methanol fuel to electrical energy, is the methanol crossover through the polymer electrolyte.2 Higher methanol tolerance
is reported in the literature for non-noble metal cathode electrocatalysts based on chalcogenides3 and macrocycles
of transition metals.4 These electrocatalysts have shown
However in methanol free electrolytes, these materials did not reach the catalytic activity of carbon supported platinum. Developing suficiently selective and active electrocatalysts for the cathodic reaction in DMFCs remains one of the tasks for further progress in this technology.
Earlier work showed that some platinum alloys with irst-row transition metals present a higher activity for the ORR than pure platinum in low temperature fuel cells operated directly with methanol.5 In general, metals such as V, Cr,
Co, Ti and Ni, alloyed with platinum exhibit signiicantly higher electrocatalytic activities for the ORR than platinum alone in low temperature fuel cells.6 These Pt-alloy
electrocatalysts improve both the cell performance and the nanoparticles resistance to sintering and coalescence under the operational conditions of the PEMFC. The enhanced ORR electrocatalysis has been ascribed to different factors such as the Pt-Pt inter-atomic distance,7 the surface area,8
the d-orbital vacancy,9 among others. Also, the observed
increase in catalytic activity for increasing Pt particle sizes has been attributed to the reduced adsorption of OH on large particles because of the change in d-band occupancy related to changes in particle size.10
Some of the problems regarding preparation methods of carbon supported Pt-M alloys are dificulty in incorporating enough quantities of non-precious metal in the alloy and increase of particle size with respect to pure Pt.11 In this
respect, electrocatalytic activity for some catalysts was found to increase with decreasing particle size,12 which was
attributed to changes in distribution of surface atoms and crystal faces or in Pt d-band occupancy.13 Maillard et al.14
found that the electrocatalytic activity of Pt/C catalysts for oxygen reduction in methanol-containing electrolytes increases when decreasing particle sizes, conversely to what they observed in methanol-free electrolytes. The mass activity for oxygen reduction in a methanol-containing electrolyte was found to increase continuously with decreasing particle size, not only because of the grater surface area of smaller particles, but also due to the existence of a signiicant particle size effect on the tolerance to methanol. This was attributed to a stronger adsorption of oxygenated species on smaller particles and to a particle shape effect modifying the methanol coverage. It has also been observed that Pt agglomeration causes a decay in catalyst mass activity owing to the decrease of platinum surface area.14
A common method of preparation of carbon supported Pt-M alloys consists in the deposition of the non-precious metal on previously formed carbon supported platinum, followed by alloying at high temperatures.15 This thermal
treatment at high temperatures (≥ 900 ºC) gives rise to an undesired metal particle growth, by sintering and coalescence of platinum particles.16
In general, when Pt-based materials incorporate a non noble metal, some non noble metal oxide may remain at the catalyst surface or may be formed during cell operation due to oxidation at high potentials. Indeed, this affects the catalyst performance. In this sense, copper is a very interesting candidate to form alloys with platinum, because copper oxide was shown to have an important role in the activity for ORR.17,18 Because few reports exist
on Pt-Cu alloys,19,20 in this work they have been prepared
and their activity tested for ORR in a DMFC. In addition, it has been observed that the introduction of Pd in some binary and ternary catalysts led to an improvement in the electrocatalytic activity for ORR.21,22 Thus, the effect of
introducing Pd into the Pt-Cu alloys was also studied under the same conditions.
Pt-Cu/C and Pt-Pd-Cu/C electrocatalysts were prepared with the addition of 0.04 mol L-1 sodium borohydride
solution on high surface area carbon (Vulcan XC-72, Cabot, 240 m2 g-1 thermally pre-treated at 850 oC under Ar
atmosphere), under sonication. Solutions of chloroplatinic acid (H2PtCl6·6H2O, Johnson Matthey), copper chloride (CuCl2·2H2O, Merck) and for the ternary catalyst, palladium chloride (PdCl2,Alfa Aesar) were slowly added to the carbon suspension. The supported catalysts were iltered, washed and dried at 80 oC in air for 1 h. The
materials were 20% m/m metal on carbon. In order to test the effect of temperature on the catalysts they were submitted to thermal treatments at 500 and 900 oC under
Ar/H2 (4:1)atmosphere for 1 h.
Energy dispersive X-ray analysis (EDX)
The mean atomic ratios of the Pt-Cu/C and Pt-Pd-Cu/C catalysts were determined by EDX technique coupled to a scanning electron microscopy LEO Mod. 440 with a silicon detector with Be window, applying 20 kV.
X-ray diffraction (XRD)
In order to estimate the mean crystallite size from XRD, Scherrer’s equation was used,23T = 0.9λ / Bcosθ, where
T is the average crystallite diameter, λ is the wavelength of the X-ray radiation (0.154056 nm), θ is the angle of the (220) peak and B is the value obtained dividing the (220) peak area by the maximum intensity. Both instrumental and strain line proile broadening were not taken into account in the calculation, assumed to be the same for all materials. Therefore, considering the comparative analysis of the present work, such approximations may not introduce signiicant errors in data analysis. The lattice parameters were obtained by reining the unit cell dimensions using FullProf program.24
Transmission electron microscopy (TEM)
The samples for the TEM characterizations were prepared as follows: a carbon ilm was deposited onto a mica sheet and after release of the ilm in water it was placed onto the Cu grids (300 mesh and 3 mm diameter). The material to be examined was dispersed in water by sonication, placed onto the carbon ilm and left to dry. This technique was implemented at the microscopy laboratory of the LNLS using a HRTEM microscope JEOL, JEM 3010, URP, operating at 300 kV, with 0.17 nm resolution.
Dispersive X-ray absorption spectroscopy (DXAS)
The use of XAS to investigate catalysts has been reviewed several times in the literature.25 The in situ X-ray
absorption time resolved spectroscopy measurements were performed at the Pt LIII absorption edge, using an appropriate spectro-electrochemical cell.26 The working
electrodes consisted of pellets formed with the dispersed catalysts compacted with a PTFE dispersion (ca. 40 wt.%) and containing 6 mg cm-2. The counter electrode was a
Pt screen. This electrode was cut in the center, in order to allow the free passage of the X-ray beam. Dispersive X-ray absorption (DXAS) experiments were done with the electrodes polarized at 0.1 V versus RHE and submitted to a linear sweep voltammetry at 10 mV s-1 from 0.1V to
1.1V versus RHE. The results presented here correspond to the time resolved X-ray absorption intensity versus the photon energy as function of potential.
Electrode preparation for cyclic voltammetry and for tests in single DMFC
Cyclic voltammetric experiments were carried out at room temperature (ca. 26 °C) in a 0.5 mol L-1 H
solution using an Ecochemie AUTOLAB PGStat 30 potentiostat. Potentials were measured using a reversible hydrogen electrode in the same solution. The working electrode was prepared by applying a thin layer (around 1 µm thickness) of the supported catalyst dispersed in water on a glassy carbon disk according to a method already described.27 Briely, a drop (approximately 45 µL)
of a re-dispersed aqueous suspension containing about 1 mg mL-1 of catalyst was dropped on top of a glassy carbon
disc of 0.348 cm2 embedded in PTFE, yielding around
56 µg Pt cm-2. After water evaporation, 40 µL of a diluted
Naion solution (0.05 wt.%, in 1:1 water/methanol) was
placed onto the dried catalyst material. The electrode was protected by a pure water droplet and then transferred to the electrochemical cell. No attempts were made to assess electrochemically the active area of the electrodes. Thus all currents were normalized by the Pt mass in the electrode (giving the so-called “mass activity”).
In order to test the electrochemical behaviour in a single DMFC fed with methanol/oxygen, the electrocatalysts were used to make two layer gas diffusion electrodes (GDE). A diffusion layer was made with carbon powder (Vulcan XCR-72R) and 15 wt.% m/m PTFE and applied over a carbon cloth (PWB-3, Stackpole). On top of this layer, the electrocatalyst was applied in the form of a homogeneous dispersion of Pt-Cu/C, Pt-Pd-Cu/C or Pt/C, Nafion®
solution (5 wt.%, Aldrich) and isopropanol (Merck). All electrodes were assembled to contain 1 mg Pt cm-2.
For the direct methanol single cells studies, the electrodes were hot pressed on both sides of a Naion® 115
membrane at 125 oC and 50 kg cm-2 for 2 min. Before using
them, the Naion® membranes were treated with a 3 wt.%
H2O2 solution, washed and then treated with a 0.5 mol L-1
H2SO4 solution. The geometric area of the electrodes was 4.6 cm2, and the anode material was 20 wt.% Pt
from E-TEK (Lot #A1160825). The cell polarization data at 70 oC / 1 atm O
2 pressure and 90
oC / 3 atm O
were obtained by circulating a 2 mol L-1 methanol aqueous
solution at the anode.
Assuming that catalyst metal particles are individual crystallites and crystallites are spheres or cubes with negligible micro porosity, the specific areas (S) were estimated using the expression: S = 6 × 103/ρd were S is
the speciic area (m2 g-1), ρ is the density (g mL-1) of the
crystallite and d is the average crystallite diameter (nm).28,29
The density of the crystallites was determined with the expression: ρ = Σj xj*ρj, were ρj is the density of metal j and x is the mass ratio in the catalyst. The densities of pure platinum, palladium and copper used were 21.45, 12.02 and 8.920 g mL-1, respectively. The speciic area calculated
However, this way of assessing the surface area gives a general idea of the surface atoms electrochemical activity while normalizing the currents with the calculated area when using the catalyst in a fuel cell. This is valid when comparing electrodes prepared in the same way. Even using the crystallite size instead of the true particle size, the approximation introduced is assumed to be the same in all cases.
Results and Discussion
The average composition of the Pt-Cu and Pt-Pd-Cu alloy catalysts was evaluated by EDX analysis. For the Pt-Cu alloys the Cu contents in various regions of the powder are considerably higher than the expected values from the precursor’s concentration ratio used in the synthesis. Conversely, the Pt content is smaller than the expected value. The nominal and EDX compositions are shown in Table 1. The EDX compositions will be used throughout this work.
Figure 1 shows the XRD patterns of the as-prepared and thermally treated carbon-supported Pt-Cu alloy catalysts with different Pt/Cu atomic ratios. As seen in Figure 1, all the XRD patterns present the main characteristic peaks of the face-centered cubic (fcc) crystalline Pt (JCPDS card, number 88-2343),30 in particular, the planes (220),
(311) and (222), showing that all the alloy catalysts mainly resemble the single-phase disordered structure (solid solution). The diffraction peaks in the Pt-Cu alloy catalysts are slightly shifted to 2θ higher values with respect to the corresponding peaks in the Pt/C catalyst.30
The shifts of the Pt peaks to higher angles reveal a lattice contraction, caused by Cu atoms incorporation, smaller than Pt atoms, in the fcc structure of Pt. The corresponding lattice parameters are shown in Table 1.
In Figure 2 the lattice parameters are plotted as a function of the Cu content (from EDX composition) showing that up to 56 at.% Cu the dependence is near linear. Thus, considering that Pt and Cu have the same crystal structure (fcc) it can be inferred that these materials follow Vegard’s law.
Table 1. Metal crystallite sizes (d) and lattice constants (a) of the Pt-Cu and Pt-Pd-Cu catalysts
Catalyst composition (Nominal ; EDX) as prepared treated at 500
oC treated at 900 oC
d (nm) a (nm) d (nm) a (nm) d (nm) a (nm)
Pt90Cu10 ; Pt70Cu30 3.2 0.391 5.7 0.390 8.0 0.389
Pt80Cu20 ; Pt60Cu40 2.7 0.389 5.1 0.388 7.7 0.386
Pt70Cu30 ; Pt50Cu50 2.6 0.387 4.8 0.385 9.9 0.383
Pt80Pd10Cu10 ; Pt60Pd20Cu20 3.2 0.389 10.2 0.388 24.8 0.386
Pt60Pd30Cu10 ; Pt50Pd40Cu10 3.3 0.389 15.1 0.388 29.3 0.387
Figure 1. XRD diffractograms of carbon supported 20 wt.% Pt-Cu/C catalysts as prepared and submitted to thermal treatment in a H2/Ar atmosphere at 500 and 900 oC. Curves a, a’ and a’’ are as prepared Pt
70Cu30, Pt70Cu30 thermally treated at 500 oC and Pt
70Cu30 thermally treated at 900 oC, respectively. Curves b, b’ and b’’ are as prepared Pt60Cu40, Pt60Cu40 treated at 500 oC and Pt
60Cu40 treated at 900
oC, respectively. Curves c, c’ and c’’ are as prepared Pt50Cu50, Pt50Cu50 treated at 500 oC and Pt
50Cu50 treated at 900 oC, respectively. The dashed vertical lines are the Bragg positions for pure Pt (JCPDS card, number 88-2343).30
The mean size of the Pt-Cu alloy crystallites was estimated from XRD using Scherrer’s equation.23 The
values are given in Table 1 and show that the mean crystallite size of the prepared Pt-Cu/C alloy catalysts falls in the range 2-3 nm, then 5-6 nm when thermally treated at 500 oC and 7-10 nm when thermally treated at 900 oC.
It is worth to note that with the increase of Cu content in the Pt-Cu catalysts the mean crystallite size decreases, and this behavior is observed even for the catalysts submitted to thermal treatment at 500 oC. On the other hand, for the
catalyst thermally treated at 900 oC the crystallite size
increases appreciably when the atomic ratio reaches 1:1. This may be due to a different temperature effect in the crystal growth in materials with high Cu contents, a subject that is beyond the scope of this work.
Considering that the catalysts studied here follow Vegard’s law, tabulated values of the lattice parameters for Pt, Pt50Cu50 and Cu, 0.39158 nm , 0.37769 nm and 0.36075 nm respectively,31 were used to calculate an “ideal” function
for the variation of the lattice parameter with the atomic percentage of Cu, at the solid solution (at.Cuss %). For this calculation we assumed a linear dependence over the full range (0-100 at.Cuss %) as the “ideal” one. The equation describing the linear dependence of the lattice parameter with the at.Cuss % at Pt:Cu compositions for which Vegard’s law is valid should be the same as the ideally calculated, independently of the occurrence of deviations at other compositions. Then, the at.Cuss % was calculated from the experimental values of the Pt-Cu catalysts lattice parameters and the Pt:Cu atomic composition of the solid solution was estimated. The resulting values are summarized in Table 2. Also, it was possible to estimate the degree of alloy and the atomic copper oxide %, as shown in Table 2.
It is clearly seen from Table 2 that the thermal treatment increases the degree of alloy, reducing the oxide content and leading to a more Cu-rich alloy in all cases. Also, it is worth to note that comparing different catalysts (i.e. with different EDX composition) some tendencies may be found. For instance, the degree of alloy increases with total Cu content (from EDX composition), but also does the copper oxide contents. This is observed for all catalysts, except for the Pt50Cu50 thermally treated at 900 oC, for which the oxide content is lower than
for the other Pt50Cu50 catalysts. Again, this may be due to a different effect of the thermal treatment for materials with high Cu content. Meanwhile, it is important to keep in mind that the thermal treatment increases the degree of alloy by reducing the oxide content, but if we compare different catalysts submitted to the same thermal treatment, a higher degree of alloy does not necessary means less oxide content. This is an important fact when electrocatalytic properties of the different catalysts are discussed.
The effect of incorporation of Pd on the diffraction patterns Figure 3 shows the XRD patterns of the as-prepared and thermally treated carbon-supported Pt-Cu catalysts that incorporate Pd. All the XRD patterns present the main characteristic peaks of the face-centered cubic (fcc) crystalline Pt, as in the case of the Pt-Cu catalysts. The diffraction peaks for the Pt-Pd-Cu alloy catalysts are slightly shifted to higher 2θ values with respect to the corresponding peaks in the Pt/C catalyst,30 indicating that
the incorporation of Cu and Pd leads to a contraction of the lattice. The lattice parameters of the Pt-Pd-Cu alloy catalysts are given in Table 1, and show that the lattice parameter decreases with the thermal treatment, indicating a reduction of oxides and alloy formation. The crystallite sizes for the Pt-Pd-Cu catalysts are shown in Table 1. Recently, it was reported that the incorporation of Pd leads to an increase in the crystallite size.21 This effect can be seen here once
the crystallite size of the thermally treated Pt50Pd40Cu10 catalyst (which has more Pd) is larger than the thermally treated Pt60Pd20Cu20 catalysts. Apparently, this indicates that the qualitative and quantitative composition of Pt based nanocrystals determines the effect of the sintering and coalescence processes under thermal treatment.
Figures 4 and 5 show TEM images for the Pt60Cu40 catalysts thermally treated at 500 and 900 oC, respectively,
and illustrate the effect of thermal treatment on morphology. They show that the metal nanoparticles are well distributed on the carbon support. In Figure 4 it can be seen that there are few large particles (larger than 15 nm) and
Table 2. Pt:Cu atomic composition as calculated by Vegard’s law, degree of alloy and copper oxide content for all the Pt-Cu catalysts
Pt-Cu catalyst / EDX composition
Pt : Cu compostition as calculated by Vegard’s law Degree of alloy/(%) Copper oxides/ (at.%)
none 96 : 4 8.3 27.5
500 93 : 7 17.0 24.9
900 90 : 10 25.9 22.2
none 90 : 10 16.7 33.3
500 87 : 13 23.0 30.8
900 80 : 20 37.0 25.2
none 83 : 17 19.8 40.1
500 77 : 23 29.9 35.1
several particles of small size (around 5 nm). On the other hand, for the Pt60Cu40 catalyst thermally treated at 900 oC
(Figure 5) there are few small particles and many large particles, in agreement with the tendency observed from the mean crystallite sizes determined from XRD, which is indicative of particle agglomeration and/or crystal growth with thermal treatment.
Considering the materials that incorporate Pd, the Pt50Pd40Cu10 catalyst thermally treated at 900o C has
larger particles than the one thermally treated at 500 oC,
as well as bigger agglomerates (10-40 nm) caused by sintering and coalescence at high temperatures (not shown). Agglomeration is an undesired consequence of high temperature thermal treatments, because it causes a decrease in the active catalyst surface area.
There is no doubt that the electronic properties of alloy catalysts are very important in determining the activity, and one of the ways to probe the electronic structure is through XAS experiments. In this work an initial evaluation of electronic effects on Pt-Cu catalysts was carried out by performing DXAS experiments with the Pt-Cu catalysts and Figure 6 shows the results for the as prepared Pt70Cu30 catalyst. The intensity of the white line is strong at low and high electrode potentials and has less intensity in the double layer region. In this region there is a minimum of adsorbed species on the electrode. At high potentials, the formation of adsorbed OH species increases on the catalyst surface, reducing the occupancy of Pt d-band which is relected in an increase of the intensity of the white line. However, in this region of high potentials the white line in the Pt70Cu30 material is not as intense as on pure platinum (not shown) which is a clear indicator that the presence of Cu in the catalyst reduces the emptying of the Pt d-band. Similar results, not shown here, were observed with the Pt60Cu40 and Pt50Cu50 catalysts. The fact that the increase in the white line is not very pronounced in the presence of Cu indicates that the catalyst has a weak tendency to form oxides as potential increases. This effect improves the ORR kinetics, because it favours molecular oxygen adsorption on a surface where the competition for surface sites is less pronounced. Ressler et al.32 showed by DXAS that the reduction of CuO/ZnO
(70 at.% Cu, 30 at.% Zn) to Cu/ZnO in an 8 vol. % H2 atmosphere is a function of the temperature, and they found that Cu is formed at around 220 oC. So, the intensity of white
line decreases when the treatment temperature is higher than 220 oC. In the present work the catalysts were thermally
treated at 500 and 900 oC in an atmosphere with 20 vol. %
of H2, and alloying was not complete, indicating that some copper remains as oxide, as can be seen in Table 2. Lee et al.17
found that PtCuO catalysts prepared by rf sputtering and used as cathode catalysts, increased the power performance of a DMFC up to 25% in comparison with that with an unmodiied Pt cathode. Also, Nabae et al.18 studied the
performance of a Cu/C cathode in a PEMFC. They proposed that the Cu2+species should function as adsorption sites for Figure 3. XRD diffractograms of carbon supported 20 wt.% Pt-Pd-Cu/C
catalysts as prepared and submitted to thermal treatment in a Ar/H2 4:1 atmosphere at 500 and 900 oC. Curves a and a’ are the Pt-Pd-Cu catalysts thermally treated at 900 oC. Curves b and b’ are the Pt-Pd-Cu catalysts thermally treated at 500 oC. Curves c and c’ are the as prepared catalysts. The dashed vertical lines are the Bragg positions for pure Pt (JCPDS card, number 88-2343).30
Figure 4. TEM micrographs of the Pt60Cu40/C catalyst prepared by chemical reduction with sodium borohydride and thermally treated at 500 oC in a Ar/H
2 4:1 atmosphere.
molecular oxygen, increasing the concentration of O2 on the cathode. These observations suggest that the presence of some Cu oxide should enhance the performance of the catalysts towards the ORR.
Figures 7 to 9 show the results of repetitive cyclic voltammetry (CV) for the three Pt-Cu catalysts submitted to thermal treatments at 500 and 900 ºC. In general, they show a similar behaviour to that observed for carbon supported Pt-based nanocatalysts, exhibiting the three main characteristic regions of hydrogen adsorption/desorption, double layer and oxide/hydroxide formation. Potential cycling induces changes in the surface structure/composition of the alloy and, as the potential is swept repeatedly between 0.05 and 1.2 V, the CV proile approaches the expected proile of carbon-supported pure platinum nanoparticles. Some small differences can be observed for the catalyst thermally treated at 900 ºC if compared to that treated at 500 ºC, specially in the hydrogen adsorption/desorption region. These differences are related to the different degree of alloy because, as XRD analysis showed, an increase in the temperature of the thermal treatment increases the degree of alloy of the catalysts and these structural differences lead to different CV proiles.
In order to evaluate and compare the activity of the Pt-Cu catalysts, tests were carried out under stationary state conditions in single direct methanol fuel cells. Being the cathode catalyst the only different element among the cells, the differences in single cell performance with different cathode catalysts relect the different activity of those catalysts toward the ORR in the presence of crossover methanol.
There are in general two ways of expressing the catalytic activity: the mass activity (MA), were the current
Figure 6. Dispersive X-ray absorption plots at the Pt edge (13564 eV) as a function of the electrode potential. From 0.1 to 1.1 V vs. RHE at 10 mV s–1.
Figure 7. Cyclic voltammograms obtained in 0.5 mol L-1 H 2SO4 at 50 mV s-1, for the Pt
50Cu50 catalysts thermally treated at (a) 500 oC and (b) 900 oC; Pt loading of 56 µg cm-2. Arrows indicate increasing number of cycles (from 5 to 20).
Figure 8. Cyclic voltammograms obtained in 0.5 mol L-1 H 2SO4 at 50 mV s-1, for the Pt
60Cu40 catalysts thermally treated at (a) 500 oC and (b) 900 oC; Pt loading of 56 µg cm-2. Arrows indicate increasing number of cycles (from 5 to 20).
Figure 9. Cyclic voltammograms obtained in 0.5 mol L-1 H 2SO4 at 50 mV s-1, for the Pt
is normalized by the Pt mass, and the speciic activity (SA), were the current is normalized by the catalyst surface area.19
The irst one has practical implications in fuel cells, since the electrode cost depends largely on the Pt contents. The second one, although the calculated area is not the real surface area, gives an idea about the electrocatalytic activity of the atoms at the surface of the catalyst. Therefore, assessing both the MA and the SA it should be possible to: i) know which catalyst has a better performance in a DMFC from a practical point of view (MA) and ii) make an approximate assessment if this is due to a better electrocatalytic activity of the surface atoms (SA) or is just due to differences in real surface area, or other effects. Although the SA values determined here are approximations, they are a useful tool when comparing materials prepared by the same method and treated under similar conditions. The values of the speciic areas (S) and the density of crystallites for the Pt-Cu catalysts are shown in Table 3.
Figures 10a and 10b show the polarization curves in terms of the SA for the as prepared and thermally treated at 500 and 900 oC Pt
70Cu30 cathode catalysts with the cell
operating at 70 and 90 oC, respectively. The results with
Pt/C are included for comparison.
The catalysts treated at 900 oC show an increase of
particle size, as discussed above, and also show the higher SA. This could be due to a particle size effect with more favorable d-band occupancy for the ORR. The observed increase in catalytic activity for the ORR when increasing particle sizes has been ascribed to the reduced strength of adsorption of oxygenated species on large particles,
because the d-band vacancy decreases. Thus, the reduction of intermediate oxygenated species on the surface of the catalyst becomes easier.14,33
The thermal treatment also has an important effect because it reduces some Cu oxides and increases the degree of alloy (Table 2). This last effect may induce a modiication of the electronic state, besides reducing de Pt-Pt distance, favoring the adsorption of molecular oxygen. Figures 11a and 11b show the polarization curves in a DMFC in terms of the SA for Pt50Cu50, as prepared and thermally treated, with the cell operating at 70 and 90 oC respectively. The catalyst
treated at 900 oC shows the best activity, as observed also for
the Pt70Cu30 catalysts. However, the effect of a larger amount of copper is not beneicial, as observed by the fact that the performance of the catalyst thermally treated at 500 oC falls
below that of Pt/C in the case of the Pt50Cu50 catalyst. From Table 2, it should be noted that, for the Pt50Cu50 catalyst thermally treated at 500 oC, the amount of copper oxides
is approximately 35 at.%. This is higher than the amount for Pt50Cu50 catalyst thermally treated at 900 oC, and for the
Pt70Cu30 catalyst thermally treated at 500 oC and 900 oC, being
their estimated content of oxides approximately 19 at.%, 25 at.% and 22 at.%, respectively.
Table 3. Density and speciic area (SA) of the catalysts
Catalyst EDX Composition
Density/ (g cm-3)
Speciic area/ (m2 g-1)
None TT 500 oC TT 900 oC
95.3 52.9 37.9
None TT 500 oC TT 900 oC
114.9 61.1 40.8
None TT 500 oC TT 900 oC
126.0 100.5 33.0
None TT 500 oC TT 900 oC
97.4 30.5 12.6
None TT 500 oC TT 900 oC
101.7 22.2 11.4
Pt/ C E-TEK 21.45 97.0
Figure 10. Cell potential vs. Current density in DMFC, in terms of SA. Cathode Pt70Cu30 as prepared; treated at 500 and 900 oC in Ar/H
Figure 11. Cell potential vs. current density in a DMFC, in terms of SA. Cathode Pt50Cu50 as prepared; thermally treated at 500 and 900 oC in Ar/H2 4:1 for 1h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Figure 12. Cell potential vs. Current density in DMFC, in terms of MA. Cathode Pt70Cu30 as prepared; thermally treated at 500 and 900 oC in Ar/H2 4:1 for 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Considering the mass activity, Figures 12a and 12b show the polarization curves in a DMFC for the Pt70Cu30 catalysts, at 70 and 90 oC respectively. The best MA was
obtained with the catalyst thermally treated at 500 oC. The
larger particle size, thus lower speciic area, for the catalyst thermally treated at 900 oC is the reason for the lower MA
for this catalyst. The as prepared catalyst, even presenting a larger speciic area, shows both a low MA and a low SA. This could be due to a greater amount of oxides present on the catalyst surface. The PtCuO catalyst prepared by Lee and co-workers17 had 8 at.% of CuO. It may be
speculated that there must be a critical amount of copper oxide beyond which the catalytic activity of the catalyst begins to decrease instead of increase. This means that the presence of low amounts of CuO on the catalyst’s surface may inhibit methanol oxidation17 and provide adsorption
sites for oxygen,18 but on the other hand, a larger amount of
these oxides on the catalyst’s surface produces a decrease in the performance of the catalyst, because the oxide covers active sites of the metal surface. The thermal treatment in a hydrogen atmosphere reduces some of the copper oxides, thus “cleaning” the surface of the catalysts.
Figures 13a and 13b show the polarization curves in a DMFC in terms of the MA for the Pt50Cu50 catalysts, at 70 and 90 oC respectively. It can be seen that in terms of MA
the performance of the Pt50Cu50 catalysts is inferior to that of Pt E-TEK. In terms of SA the Pt50Cu50 thermally treated at 900 oC catalyst shows a better activity than Pt/C (Figure 11),
probably due to a particle size effect, an electronic effect (related to the irst one), a more favorable Pt-Pt distance, and/or a smaller copper oxide content. However, the speciic area is too small, so the MA for this catalyst is very low. The Pt60Cu40 catalysts showed a behavior similar to that of the Pt50Cu50 and the results are not shown here.
For all the Pt:Cu compositions, the best values of MA (the ones of practical relevance) were obtained with the catalysts thermally treated at 500 oC. Figures 14a and 14b
and 15a and 15b show the effect of the Cu content in the catalysts treated at 500 oC in terms of both SA (Figure 14)
DMFC for the thermally treated (T = 500 oC) catalysts
is shown, in terms of MA, in Figure 16 as a function of Cu content. The best performance is observed for the Pt70Cu30 catalyst, but this is similar to that of pure Pt, for both 70 and 90 oC.
As in the case of the Pt-Cu catalysts, the best performance in terms of MA (the one of practical importance) of the cathode catalysts incorporating palladium was obtained with those catalysts thermally treated at 500 oC, and the polarization
curves obtained for the other catalysts are not shown. Figures 17a and 17b show the polarization curves in terms of MA for the Pt-Pd-Cu catalysts thermally treated at 500 oC. It can be seen from Figure 17 that the best
performance was obtained with the Pt50Pd40Cu10 catalyst, even though the speciic area of this catalyst is smaller than that of the Pt60Pd20Cu20 catalyst thermally treated at the same temperature. Figures 18a and 18b show the polarization curves in terms of the SA for the Pt-Pd-Cu catalysts thermally treated at 500 oC. The Pt
50Pd40Cu10 catalyst shows
the best performance in terms of SA, and that is why it has
a better MA even though it has a smaller speciic area than the Pt60Pd20Cu20 catalyst. As the lattice parameter is similar for both catalysts (0.388 nm) the difference in activity can be attributed to differences in the electronic state and/or to different copper oxide contents.
It was mentioned above that the presence of some copper oxide in the catalysts can hinder methanol oxidation and favor the adsorption of molecularoxygen, improving the performance of the catalyst as cathode material in a DMFC. This, along with the electronic effects arising from the introduction of Cu and Pd into the alloy, may be the reason for the better performance of this Pt-Pd-Cu catalyst than pure Pt. To evaluate the differences between the Pt-Cu and Pt-Pd-Cu catalysts, the polarization curves with the Pt60Cu40 and Pt60Pd20Cu20 catalysts in the cathode, both thermally treated at 500 oC are compared in Figures 19a and 19b at 70
and 90 oC, respectively, in terms of SA. These two catalysts
were chosen for comparison because they have a similar Pt content (approximately 60 at.%), similar lattice parameter (Table 1) and both have probably a similar dispersion on the carbon support since they were both prepared by the same method and thermally treated at the same temperature.
Figure 13. Cell potential vs. current density in a DMFC, in terms of MA. Cathode Pt50Cu50 as prepared; thermally treated at 500 and 900 oC in Ar/H2 4:1 for 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Figure 15. Cell potential vs. Current density in a DMFC, in terms of MA. Cathode Pt50Cu50; Pt60Cu40 and Pt70Cu30 thermally treated at 500 oC in Ar/H2 4:1 for 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Figure 16. Effect of Cu content in the maximum power density of DMFCs, in terms of the MA at 70 oC and 90 oC. Anode Pt
50Ru50 from E-TEK. 1 mol L-1 methanol.
They were chosen also because in all cases the best performance was obtained with the catalysts thermally treated at 500 oC. Thus, differences in performance can be
attributed to particle size effects (different active surface area), electronic effects and/or differences in copper oxide content. It can be seen from Figure 19 that the Pt60Pd20Cu20
Figure 17. Cell potential vs. Current density in a DMFC, in terms of MA. Cathode Pt60Pd20Cu20 andPt50Pd40Cu10 thermally treated at 500 o C in Ar/H2 4:1 for 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
catalyst has a much better SA than the Pt60Cu40 catalyst. This is probably due to an electronic effect and to the presence of more copper oxide in the Pt60Cu40 catalyst. Figures 20a and 20b show the polarization curves in terms of MA for the same two catalysts. Even though the speciic area of the Pt60Pd20Cu20 catalyst is almost half of that of the Pt60Cu40 catalyst, it shows a better performance in terms of the MA. This means that the better SA of the ternary catalyst compensates the fact that it has a larger particle size (thus, a smaller surface area), which results in a better MA. Still, it is not clear if this improvement comes from an electronic effect, a different copper oxide content, or both, which have a favorable effect on ORR activity and on the tolerance to methanol. It is clear that more detailed studies will have to be carried out.
at 900 oC increases too much the particle size when the
atomic ratio Pt:Cu reaches 1. The crystallite size decreases linearly with the increase of Cu content in the catalysts, but this effect is not decisive for the performance of the catalyst as a cathode in the DMFC. The amount of copper in the alloyed form and in the oxide form, carefully balanced, seems to be more important.
The incorporation of Pd in addition to Cu to Pt resulted in an improvement of the fuel cell performance, being the Pt50Pd40Cu10 catalyst thermally treated at 500 oC the one who
showed the best performance in terms of MA, probably due to electronic effects and because, at the thermal treatment temperature, some copper oxide is reduced without the formation of agglomerates.
The comparison of the DMFC performances with cathode catalysts with different Pd/Cu ratio shows that the material with higher noble metal content (Pt+Pd) performs better, following the tendency observed with the Pt-Cu binary catalysts. Also, the comparison between a PtCu and a Pd-modiied PtCu cathode with the same Pt content showed the same tendency, i.e. having the Pd-modiied PtCu cathode a better performance in a DMFC. All this supports previous indings showing that the incorporation of Pd in a cathode catalyst improves the activity for the ORR and the tolerance to methanol.
Figure 18. Cell potential vs. current density in a DMFC, in terms of SA. Cathode Pt60Pd20Cu20 andPt50Pd40Cu10 thermally treated at 500 o C in Ar/H2 4:1 by 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Figure 19. Cell potential vs. current density in a DMFC, in terms of SA. Cathode Pt60Pd20Cu20 and Pt60Cu40 thermally treated at 500 oC in Ar/H
2 4:1 for 1 h. Anode Pt50Ru50 from E-TEK. 1 mol L-1 methanol. (a) 70 oC; (b) 90 oC.
Supplementary data are available free of charge at http://jbcs.sbq.org.br, as PDF ile.
The authors thank, the Conselho Nacional de Desenvolvimento Cientíico e Tecnológico (CNPq) and Fundação de Amparo a Pesquisa do Estado de São Paulo, (FAPESP) for inancial assistance to the project. Thanks are also due to the Brazilian Synchrotron Light Laboratory (LNLS, Campinas, SP, Brazil) for the use of the beam line D06A-DXAS, D12A-DRX1 and HR-TEM.
1. Löfler, M.-S.; Natter, H.; Hempelmann, R.; Wippermann, K.;
Electrochim. Acta 2003, 48, 3047.
2. Yang, B.; Manthiram, A.; Electrochem. Commun. 2004,6, 231. 3. Schmidt, T. J.; Paulus, U. A.; Gasteiger, H. A.; Alonso-Vante,
N.; Behm, R. J.; J. Electrochem. Soc.2000, 147, 2620. 4. Baranton, S.; Coutanceau, C.; Leger, J-M.; Roux, C.; Capran,
P.; Electrochim. Acta2005, 51, 517.
5. Antolini, E.; Salgado, J. R. C.; Gonzalez, E. R.; Appl. Catal., B
2006, 63, 137.
6. Yang, H.; Alonso-Vante, N.; Léger, J-M.; Lamy, C.; J. Phys. Chem. B 2004, 108, 1938.
7. Russell, A. E.; Maniquet, S.; Mathew, R. J.; Yao, J.; Robert, M. A.; Thompsett, D.; J. Power Sources 2001, 96, 226.
8. Antolini, E.; Mater. Chem. Phys.2003, 78, 563.
9. Santiago, E. I.; Giz, M. J.; Ticianelli, E. A.; J. Solid State Electrochem. 2003, 7, 607.
10. Teliska, M.; Murthi, V. S.; Mukerjee, S.; Ramaker, D. E.;
J. Electrochem. Soc. 2005, 152, A2159.
11. Antolini, E.; J. Appl. Electrochem. 2004, 34, 563.
12. Min, M-k.; Cho, J.; Cho, K.; Kim, H.; Electrochim. Acta2000,
13. Antolini, E.; Salgado, J. R. C.; Giz, M. J.; Gonzalez, E. R.; Int. J. Hydrogen Energy 2005,30, 1213.
14. Maillard, F.; Martin, M.; Gloaguen, F.; Léger, J.-M; Electrochim Acta 2002, 47, 3431.
15. Carmo, M.; Paganin, V. A.; Rosolen, J. M.; Gonzalez, E. R.;
J. Power Sources 2005, 142, 169.
16. Beard, C.B.; Ross, P.N.; J. Electrochem. Soc. 1990,137, 3368.
17. Lee, J. K.; Choi, J.; Kang, S. J.; Lee, J. M.; Tak, Y.; Lee, J.;
Electrochim Acta2007, 52, 2272.
18. Nabae, Y.; Yamanaka, I.; Otsuka, K.; Appl. Catal. A2005, 280, 149.
19. Tseng, C.-J.; Lo, S. –T.; Lo, S. –C.; Chu, P. P.;Mater. Chem. Phys.2006, 100, 385.
20. Xiong, L.; Kannan, A.M.; Manthiram, A.; Electrochem. Commun. 2002, 4, 898; Stassi, A.; D’Urso, C.; Baglio, V.;
Di Blasi, A.; Antonucci, V.; Aricò, A. S.; Castro Luna, A. M.; Bonesi, A.; Triaca, W. E.; J. Appl. Electrochem.2006, 36, 1143; Liu, J. H.; Jeon, M. K.; Woo, S. I.; Appl. Surf. Sci.2006, 252, 2580; Baglio, V.; Stassi, A.; Di Blasi, A.; D’Urso, C.; Antonucci, V.; Aricò, A. S.; Electrochim. Acta2007, 53, 1360.
21. Zhang, L.; Lee, K. C; Zhang, J.; Electrochim. Acta 2007,52, 3088.
22. Mustain, W. E.; Kepler, K.; Prakash, J.; Electrochim Acta
2007, 52, 2102; Raughuveer, V.; Ferreira, P. J.; Manthiram,
A.; Electrochem. Commun. 2006,8, 807; Tarasevich, M. R.;
Chalykh, A.E.; Bogdanovskaya, V. A.; Kuznetsova, L. N.; Kapustina, N. A.; Efremov, B. N.; Ehrenburg, M. R.; Reznikova, L. A.; Electrochim. Acta2006, 51, 4455.
23. Salgado, J. R. C.; Antolini, E.; Gonzalez, E. R.;J. Power Sources
2005, 141, 13.
24. Rodríguez-Carbajal, J.; Phys. B1993, 192, 55.
25. Mukerjee, S.; Srinivasan, S.; Soriaga, M.; McBreen, J.; J. Phys. Chem. 1995,99, 4577.
26. Mukerjee, S.; Srinivasan, S.; Soriaga, M. P.; McBreen, J.;
J. Electrochem. Soc. 1995, 142, 1409.
27. dos Santos, L.; Colmati, F.; Gonzalez, E. R.; J. Power Sources,
2006, 159, 867.
28. Travitsky, N.; Ripenbein, T.; Golodnitsky, D.; Rosenberg, Y.; Burshtein, L.; Peled, E.; J. Power Sources2006, 161, 782. 29. Antolini, E.; Salgado, J. R. C.; Gonzalez, E. R.; J. Electroanal.
Chem.2005, 508, 145.
30. International Center for Diffraction Data, ICDD, PDF2 database.
31. Schneider, A.; Esch, U.; Z. Elektrochem. 1994,50, 290. 32. Ressler, T.; Wienold, J.; Jentoft, R. E.; Neisius, T.; Günter, M.
M.; Top. Catal.2002, 1-2, 45.
33. Min, M.; Cho, J.; Cho, K.; Kim, H.; Electrochim Acta 2000,
Received: January 19, 2009
Web Release Date: December 3, 2009
Supplementary Information0103 - 5053 $6.00+0.00
#Present address: Instituto de Química, Campus Samambaia, UFG, CP
131, 74001-970 Goiânia - GO, Brazil
Pt-Cu/C and Pd Modiied Pt-Cu/C Electrocatalysts for the Oxygen Reduction
Reaction in Direct Methanol Fuel Cells
Emilia A. Carbonio, Flavio Colmati,# Eduardo G. Ciapina, Maristela E. Pereira and
Ernesto R. Gonzalez*
Instituto de Química de São Carlos, Universidade de São Paulo, CP 780, 13560-970 São Carlos - SP, Brazil
Figure S1. TEM micrographs of the Pt60Cu40/C catalyst prepared by chemical reduction with sodium borohydride and thermally treated at 500 oC in an
Ar/H2 4:1 atmosphere.
Figure S2. TEM micrograph of the Pt60Cu40/C catalyst prepared by chemical reduction with sodium borohydride and thermally treated at 900 oC in an
Figure S3. TEM micrograph of the Pt50Pd40Cu10/C catalyst prepared by chemical reduction with sodium borohydride and thermally treated at 500 oC in
an Ar/H2 4:1 atmosphere.
Figure S4. TEM micrograph of the Pt50Pd40Cu10/C catalyst prepared by chemical reduction with sodium borohydride and thermally treated at 500 oC in
an Ar/H2 4:1 atmosphere.
Figure S5. Cyclic voltammogram obtained in 0.5 mol L-1 H
2SO4 at 50 mV s
-1, for the Pt
60Pd20Cu20 and Pt50Pd40Cu10 catalysts thermally treated at 900